A dynamic mechanical method for determining the silicone elastomer
solubility of drugs and pharmaceutical excipients in silicone
intravaginal drug delivery rings
Malcolm, R. K., McCullagh, S., Catney, M., Tallon, P., & Woolfson, D. (2002). A dynamic mechanical method for determining the silicone elastomer solubility of drugs and pharmaceutical excipients in silicone intravaginal drug delivery rings. DOI: 10.1016/S0142-9612(02)00086-8
Published in: Biomaterials
Publisher's PDF, also known as Version of record
Queen's University Belfast - Research Portal:
Link to publication record in Queen's University Belfast Research Portal
Copyright for the publications made accessible via the Queen's University Belfast Research Portal is retained by the author(s) and / or other copyright owners and it is a condition of accessing these publications that users recognise and abide by the legal requirements associated with these rights.
Take down policy
The Research Portal is Queen's institutional repository that provides access to Queen's research output. Every effort has been made to ensure that content in the Research Portal does not infringe any person's rights, or applicable UK laws. If you discover content in the Research Portal that you believe breaches copyright or violates any law, please contact firstname.lastname@example.org.
A dynamic mechanical method for determining the silicone elastomer
solubility of drugs and pharmaceutical excipients in silicone
intravaginal drug delivery rings
R. Karl Malcolm*, Stephen McCullagh, A. David Woolfson, Martin Catney, Paul Tallon
School of Pharmacy, The Queen’s University of Belfast, Medical Biology Centre, 97 Lisburn Road, Belfast BT9 7BL, Northern Ireland, UK Received 21 August 2001; accepted 28 February 2002
The silicone elastomer solubilities of a range of drugs and pharmaceutical excipients employed in the development of silicone intravaginal drug delivery rings (polyethylene glycols, norethisterone acetate, estradiol, triclosan, oleyl alcohol, oxybutynin) have been determined using dynamic mechanical analysis. The method involves measuring the concentration-dependent decrease in the storage modulus associated with the melting of the incorporated drug/excipient, and extrapolation to zero change in storage modulus. The study also demonstrates the effect of drug/excipient concentrations on the mechanical stiffness of the silicone devices at 371C. r 2002 Elsevier Science Ltd. All rights reserved.
Keywords: Silicone elastomer solubility; Intravaginal rings; Dynamic mechanical analysis
Silicone intravaginal rings (IVRs) are elastomeric, torus-shaped drug delivery devices (Fig. 1) designed to release drug(s) to the vagina [1–3]. The rings have, to date, been primarily developed for the systemic delivery of contraceptive steroids [1,4–7] and the localized and systemic delivery of steroids for hormone replacement therapy [1–3,8–10], although it is likely they will in the future be exploited for a much wider range of applications within women’s health care including the delivery of anti-infective agents and HIV microbicides. Unsurprisingly, the IVR, which was specifically designed for the intravaginal administration of drugs, overcomes many of the disadvantages associated with more traditional vaginal drug dosage forms, such as gels, tablets and pessaries, which are often difﬁcult to apply, interfere with intercourse and are poorly retained within the vagina . However, the major advantage of the IVR is its ability and versatility in providing long-term, continuous release of drug(s) at constant pre-determined rates, thereby increasing cost-effectiveness, patient compliance and therapeutic efﬁcacy .
Several designs of IVR have been developed, includ-ing matrix, reservoir and shell-type variants, each providing very different drug release proﬁles [1,4,11]. As with all diffusion/permeation-controlled delivery systems, the two major parameters inﬂuencing drug release rates from IVRs are the solubility and diffusivity of the drug in the silicone elastomer [1,3,12]. For example, Eqs. (1) and (2) model the release of drug under sink conditions from matrix- and reservoir-type IVRs, respectively, where Q is the release per unit area, t is time, A is the drug loading per unit volume in a matrixdevice, DSIL is the effective silicone diffusion coefﬁcient of the drug, CSIL is the silicone solubility of the drug, and h is the thickness of the sheath layer in a reservoir device
Q ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃDSILð2A CSILÞCSILt p
h : ð2Þ
These equations have been used to determine the silicone diffusion coefﬁcient of certain steroidal drugs for intravaginal administration [3,13]. Brieﬂy, a linear Q versusOt or t release proﬁles is plotted whose gradient is a function of both DSIL and CSIL: Thus, if CSIL is known, DSIL can be determined easily. However, there are practical difﬁculties associated with directly
*Corresponding author. Tel: 44-028-9027-2319; fax: 44-028-9024-779.
E-mail address:email@example.com (R.K. Malcolm).
0142-9612/02/$ - see front matter r 2002 Elsevier Science Ltd. All rights reserved. PII: S 0 1 4 2 - 9 6 1 2 ( 0 2 ) 0 0 0 8 6 - 8
measuring the solubility of a species in a polymeric network. Unlike simple saturated solutions, it is impossible to ﬁlter the excess material from a drug-saturated polymer network. For this reason, approx-imation techniques are commonly employed. For example, the solubility of drugs in low molecular weight silicone oils has been widely used as an approximation to silicone elastomer solubility [3,13,14]. However, there are inevitably some compromises associated with this indirect approach to solubility determination. It is common practice to incorporate various quantities of ﬁnely ground ﬁllers, such as diatomaceous earth, into silicone elastomers for IVR manufacture to improve their mechanical properties. The presence of ﬁllers is known to decrease the effective silicone diffusion coefﬁcient of steroidal drugs in silicone matrices as a result of the Langmuir adsorption of molecules onto the ﬁller particles [15–17]. Also, drug solubility is expected to depend on both the network chain length and the degree of cross-linking. Clearly, these factors are not taken into account in the silicone oil solubility methodology.
In an attempt to overcome some of these compro-mises, alternative direct methods for determination of drug solubility in a silicone elastomer are required. Theeuwes at al. described a now widely used differential scanning calorimetry method for determining quantita-tively the concentration of progesterone and cholesterol at their melting point in polydimethylsiloxane rubber . Here we report a novel application of dynamic mechanical analysis (DMA) in the determination of silicone solubilities for a range of drugs and pharma-ceutical excipients.
2. Experimental 2.1. Materials
Silicone elastomer base MED-6382, consisting of a mixture of high (10,000 Da) and low (2000 Da) mole-cular weight a,o-hydroxy terminated
poly(dimethyl-siloxanes), a reinforcement ﬁller (diatomaceous earth), a low molecular weight polydimethylsiloxane processing ﬂuid (to modify viscosity for injection molding pur-poses), and tetrapropoxysilane (TPOS) were obtained from Nusil Technology (Carpinteria, USA). Stannous 2-ethyl-hexanoate (stannous octoate), 17b-estradiol (E2), oleyl alcohol (OA) and norethisterone acetate (NetAc) were purchased from Sigma (UK). Poly(ethyleneglycol)s (PEG) 1000, 2000 and 6000 and poly(dimethylsiloxane) 200s
ﬂuid were purchased from Aldrich (UK). Triclo-san (TRIC) was purchased from CIBA Speciality Chemicals plc and oxybutynin free-base (OXY) was supplied by Orgamol (Evionnaz, Switzerland). All materials were used as received.
2.2. Preparation of the silicone strips
A 2 kg batch of the silicone elastomer mixwas prepared by thoroughly mixing 2.5 parts by weight of TPOS with 100 parts of MED-6382 silicone elastomer base in a Kenwood Major food mixer for 30 min. Each of the following drugs or pharmaceutical excipients (polyethylene 6000, polyethylene glycol 2000, polyethy-lene glycol 1000, oxybutynin, triclosan, oleyl alcohol, norethisterone acetate, 17b-estradiol) was then hand-blended into 35 g samples of the silicone elastomer mix at various concentrations (1–20%, Table 1) to produce the active elastomer mix, which was then allowed to stand overnight to remove air entrapped during blend-ing. One percent by weight of the curing catalyst, stannous 2-ethyl-hexanoate, was then added dropwise to the active silicone mixes and mixed for 30 s with a glass rod before injecting the mixes via a disposable 60 ml concentric-tipped plastic syringe into a specially manu-factured aluminum mold of dimensions 12.75 3.12 200 mm. The dimensions of the mold were chosen to match the sample constraints of the three-point bend clamp of the dynamic mechanical analyzer. The mold was placed in a pre-heated oven (801C) for 5 min to allow the active silicone mixto cure. These conditions were selected to mimic a typical IVR manufacturing process. The cured elastomer strip was then removed from the mold, cut into sections approximately 30 mm in length and stored for 1 week at ambient conditions in preparation for DMA analysis.
2.3. Dynamic mechanical characterization
DMA is a technique that is employed in the structural analysis of viscoelastic materials, that is, materials displaying both elastic and dissipative components of deformation. The technique involves applying an oscillatory strain wave to a sample which results in an oscillatory stress response with a phase lag (d) in between which is a measurement of the viscous contribution. A DMA 2980 dynamic mechanical
Fig. 1. Matrix-type silicone intravaginal ring. Dimensions: 54 mm external diameter, 9 mm cross-sectional diameter.
R.K. Malcolm et al. / Biomaterials 23 (2002) 3589–3594 3590
analyzer (TA instruments, Leatherhead, UK) was used to characterize the mechanical properties of the drug/ excipient-loaded silicone strips. The silicone elastomer strips were mounted on a 3-point bend clamp, as illustrated in Fig. 2, the distance between the ﬁxed clamp support bars being 20.00 mm. The sample was then periodically deformed using a static force of 0.010 n, an oscillatory amplitude of 200 mm, an oscilla-tory frequency of 1 Hz and an autotension of 150%. The autotension is the percentage of the static force needed to statically deform the sample by an amount equal to the oscillation amplitude. After establishing a reprodu-cible response at ambient temperature, the sample was heated at 21/min over a broad temperature range encompassing 371C and the melt temperature of the drug/excipient. Three repetitions were made for each strip. The parameters measured were storage modulus (G0), loss modulus (G00) and tan d:
2.4. Solubility of excipients/drugs in low molecular weight polydimethylsiloxane fluid
The silicone solubility of the ultraviolet-active drugs/ excipients (norethisterone acetate, estradiol and oxybu-tynin) was determined in triplicate according to a previously described UV-HPLC method . Brieﬂy, approximately 100 mg of each drug was added to 3.0 ml of poly(dimethylsiloxane) 200s ﬂuid. After equilibra-tion for 48 h at 371C in an orbital shaker (Model
10 400.XX2.C, Sanyo Gallenkamp, Uxbridge,UK; 60 rpm, 32 mm orbit diameter) the saturated solutions were ﬁltered at 371C (Nalgene cellulose acetate ﬁlters, 0.2 mm) and 1.0 ml of the ﬁltrate extracted into 100 ml acetonitrile. Drug solubilities in silicone were then determined by reverse phase HPLC. The Shimadzu HPLC system consisted of a model SIL-10AXL auto injector, a model SCL-10A system controller, a model LC-10AT solvent delivery module, a model FCV-10AL low pressure gradient ﬂow valve, a model GT-154 degassing unit, a model SPD-10A uv-vis detector and a
Melting points and changes in storage modulus observed in the dynamic mechanical plots of storage modulus vs. temperature Drug/excipient Mean7SD of observed
melting point (1C)
Change in storage modulus DG0(MPa) (standard deviation, n ¼ 3)
% drug excipient concentration
1 2 5 7.5 10 15 20 PEG 6000 65.770.7 1.72 4.21 7.81 (0.27) (0.30) (0.57) PEG 2000 55.375.0 0.09 1.04 2.64 4.63 (0.02) (0.17) (0.12) (0.19) PEG 1000 35.47 1.5 0.06 0.27 0.60 2.07 (0.02) (0.04) (0.05) (0.18) Oxybutynin 59.071.0 a 0.10 1.68 3.20 6.58 (0.01) (0.23) (0.19) (0.46) Triclosan 62.272.1 a 0.61 1.84 5.08 (0.07) (0.45) (0.30) Oleyl Alcohol 7.072.7 0.02 0.45 1.05 2.68b (0.01) (0.09) (0.07) (0.16) Norethisterone Acet. 153.572.8 a 1.21 3.53 8.04 (0.15) (0.40) (0.42) Estradiol 176.074.4 1.52 1.87 4.37 7.29 (0.10) (0.22) (0.35) (0.27) a
No decrease in storage modulus observed for this sample. b
9.4% oleyl acohol.
4.6 mm i.d. 150 mm Luna 5 mm C18 column (Phenom-enex, Cheshire, UK). HPLC analysis was performed at ambient temperature in isocratic mode, using an acetonitrile/pH 5 acetate buffer mobile phase delivered at 1.5 ml/min and 10 ml injection volumes. Speciﬁc parameters relating to each assay are: norethisterone acetate—85/15 mobile phase, 220 nm detection wave-length, 2.2 min retention time; estradiol—50/50 mobile phase, 281 nm detection wavelength, 2.0 min retention time; oxybutynin—45/55 mobile phase, 220 nm detec-tion wavelength, 2.0 min retendetec-tion time. The silicone solubilities of each drug were calculated using linear calibration curves produced by plotting peak areas versus concentration for a range of stock calibration solutions prepared in acetonitrile.
3. Results and discussion
Dynamic mechanical analysis is a versatile technique that may be used to simultaneously characterize both the mechanical and thermal properties of a wide range of polymeric materials of pharmaceutical and biomedi-cal signiﬁcance . To date, it has been used to measure glass transition temperature, blend compatibility, me-chanical moduli, damping properties and rates of curing. In this study, a novel DMA method for determination of the silicone elastomer solubility of a range of drugs and pharmaceutical excipients at their melting point is reported. The drugs chosen represent examples of therapeutic agents currently being evaluated for IVR development [1–4,8–10], while the choice of excipients includes materials being investigated in our laboratory for modifying drug release from the rings.
Representative plots of storage modulus vs. tempera-ture are shown in Figs. 3 and 4 for NetAc and PEG 6000-loaded silicones, respectively. The other drug/ excipient-loaded silicone samples produced similar plots. At higher drug/excipient loadings, G0 is observed to decrease sharply at the drug/excipient melting point. Table 1 provides a summary of the mean decrease in storage moduli (DG0) at the melt temperature for those samples in which it is observed. The coefﬁcient of variation for the triplicate DG0measures waso25% for all samples, and typically o12%. Fig. 5 shows repre-sentative plots of DG0 vs. drug/excipient concentration for NetAc and PEG 6000-loaded silicones. Table 2 summarizes this information for all samples. The effect of drug/excipient concentration on the storage modulus at 371C is shown in Fig. 6.
In Figs. 3 and 4, the effects on G0 (a measure of the ‘stiffness’ of a material) of incorporating various concentrations of norethisterone acetate and polyethy-lene glycol 6000, respectively, are aptly demonstrated. The blank silicone matrixshows an increase (4.3–6.0 MPa) in G0 over the temperature range. On
0 2 4 6 8 10 12 20 40 60 80 100 120 140 160 180 200
Storage Modulus (MPa)
of NetAc-loaded silicone strip
20% NetAc 10% NetAc
5% NetAc 1% NetAc
Fig. 3. Storage modulus as a function of norethisterone acetate concentration and temperature.
0 2 4 6 8 10 12 20 40 60 80 100 120 140
Storage Modulus (MPa)
of PEG-loaded silicone strip
20% PEG 10% PEG 5% PEG Blank Silicone
Fig. 4. Storage modulus as a function of polyethylene glycol 6000 concentration and temperature.
y = 0.40x - 0.08 y = 0.4547x - 1.045 R2 = 0.99 R2 = 0.9999 0 1 2 3 4 5 6 7 8 9 0 5 10 15 20
Change in storage modulus
at melting point (MPa) NetAc PEG 6000
Drug/Excipient Concentration (%w/w)
Fig. 5. Melt-associated decrease in storage modulus as a function of drug/excipient concentration for norethisterone acetate (NetAc) and polyethylene glycol 6000 (PEG 6000).
R.K. Malcolm et al. / Biomaterials 23 (2002) 3589–3594 3592
incorporation of 1% NetAc into the silicone elastomer, a similar trend when shifted to higher G0 values is observed. The increase in G0 with increasing NetAc concentration is also observed for the 5%, 10% and 20% NetAc samples. However, unlike the 1% sample, a discontinuity is observed at approximately 1601C in each plot, a temperature corresponding to the melt temperature of NetAc. The discontinuity cannot be attributed to any thermo-mechanical transitions of the silicone elastomer, as evidenced by the linear modulus– temperature plot for the blank silicones (Figs. 3 and 4). The insensitivity of storage modulus to temperature has been noted previously for silicone elastomeric denture soft lining materials . Poly(dimethylsiloxane)s typi-cally display a glass transition, a crystallization transi-tion and a melting transitransi-tion at approximately 1201C, 901C and 401C, respectively .
The magnitude of the discontinuity, as represented by the decrease in G0 (Table 1), is clearly linearly propor-tional to the concentration of NetAc in the silicone elastomer (Table 2 and Fig. 5). Thus, in the 1% NetAc sample, all of the drug must be solubilized within the
silicone elastomer near the melt temperature, since no melt-associated decrease in G0 of the silicone elastomer is observed. At higher NetAc concentrations, a fraction of the drug remains undissolved giving rise to a concentration-dependent decrease in G0 on melting.
By plotting DG0 vs. NetAc concentration (Fig. 5), a straight-line relationship is observed whose x-axis intercept corresponds to the solubility of the drug in the silicone elastomer at the melt temperature. Similar linear, best-ﬁt plots are observed for the other drug/ excipient samples investigated (r2> 0:96), producing silicone elastomer solubilities of between 1.9 and 23 mg/g. These values are comparable with those obtained for cholesterol (35 mg/g, melting point 1311C) and progesterone (6 mg/g, melting point 1291C) using a related differential scanning calorimetry method . Estradiol, whose exceptionally poor silicone solubility has prevented the development of an IVR capable of providing the clinically desired >50 mg/day release rate required for estrogen replacement therapy [1–3], shows a negative solubility value (1.21 mg/g, Table 2) as determined by the dynamic mechanical method. Such a negative value demonstrates the difﬁculty in using this technique for substances with very poor silicone solubility.
It is important to realize that the solubilities measured according to this dynamic mechanical method only apply at the melting point of the substance under investigation. Thus, for the high melting point drugs the calculated solubility is typically several orders of magnitude greater than the solubility determined in silicone oil at 371C (Table 2). However, for the lower melting oxybutynin the DMA solubility value of 15.6 mg/g at 591C relates well to 10.7 mg/g measured at 371C in silicone oil.
In addition to the quantiﬁcation of silicone elastomer solubilities, the results of the present study also demonstrate the effect of drug/excipient concentrations upon the mechanical properties of silicone devices. At body temperature, the two liquid excipients, PEG 1000 and oleyl alcohol, do not show the increasing stiffness (G0) associated with increasing concentration of the 2 4 6 8 10 12 0 5 10 15 20 % w/w concentration of drug/excipient
Mean Storage Modulus at 37
o C OXY TRIC OA NETAC E2 PEG6000 PEG2000 PEG 1000
Fig. 6. Inﬂuence of drug/excipient concentration on the magnitude of the storage modulus of silicone elastomer at 371C.
Silicone elastomer and silicone oil solubilities of drugs and excipients
Drug/excipient Gradient of best ﬁt line R2coefﬁcient X-axis intercept
(solubility at mp, mg/g)
Mean silicone oil solubility7SD (mg/g) PEG 6000 0.40 0.99 1.9 — PEG 2000 0.49 0.98 1.9 — PEG 1000 0.22 0.96 11 — Oxybutynin 0.50 1.00 15.6 10.69670.833 Triclosan 0.57 0.99 12.5 — Oleyl alcohol 0.31 0.99 9.3 — Norethisterone acet. 0.46 1.00 23 0.62270.041 Estradiol 0.66 0.99 1.21 0.00470.001
higher melting drugs/excipients (Fig. 6). In fact, increas-ing the PEG 1000 concentration has little inﬂuence on G0; while increasing oleyl alcohol concentration shows a signiﬁcant decrease in G0:
A novel dynamic mechanical method for determining the solubilities of drugs and pharmaceutical excipients in silicone elastomeric drug delivery devices is reported. The method has obvious advantages over other approx-imation methods in that the solubility is measured directly in the elastomer and thus includes effects associated with molecular weight, cross-linking density and the presence of ﬁller. The disadvantage is solubility determination is measured at the drug/excipient melting point, rather than at body temperature. However, for drugs such as oxybutynin, similar values were obtained using the dynamic mechanical method and the silicone oil approximation method, suggesting that the dynamic mechanical method is well suited to substances whose melting point is close to body temperature.
 Woolfson AD, Malcolm RK, Gallagher R. Drug delivery by the intravaginal route. Crit Rev Ther Drug Carr System 2000;17: 509–55.
 Woolfson AD, Elliot GRE, Gilligan CA, Passmore CM. Design of an intravaginal ring for the controlled delivery of 17b-estradiol as its 3-acetate ester. J Control Rel 1999;61:319–28.
 Russell JA, Malcolm RK, Campbell K, Woolfson AD. High performance liquid chromatographic determination of 17b-estradiol and 17b-17b-estradiol-3-acetate solubilities and diffusion coefﬁcients in silicone elastomeric intravaginal rings. J Chrom B 2000;744:157–63.
 Mishell DR. Vaginal contraceptive rings. Ann Med 1993;25: 191–7.
 Sivin I, Diaz S, Croxatto HB, Miranda P, Shaaban M, Sayed E, Xiao B, Wu SC, Du MK, Alvarez F, Brache V, Basnayake S, McCarthy T, Lacarra M, Mishell DR, Koetsawang S, Stern J, Jackanicz T. Contraceptives for lactating women: a comparative
trial of a progesterone-releasing vaginal ring and the copper T 380A IUD. Contraception 1997;55:225–32.
 Chen JH, Wu SC, Shao WQ, Zou MH, Hu J, Cong J, Miao L, Wang C, Dong J, Gao J, Xiao BL. The comparative trial of TCu 380A IUD and progesterone-releasing vaginal ring used by lactating women. Contraception 1998;57:371–9.
 Massai R, Miranda P, Valdes P, Lavin P, Zepeda A, Casado ME, Silva MA, Fetis G, Bravo C, Chandia O, Perlata O, Croxatto HB, Diaz S. Preregistration study on the safety and contraceptive efﬁcacy of a progesterone-releasing vaginal ring in Chilean nursing women. Contraception 1999;60:9–14.
 Henriksson L, Stjernquist M, Boquist L, Cedergren I, Selinus I. A one-year mutlicenter study of efﬁcacy and safety of a continuous, low-dose, estradiol-releasing vaginal ring (Estring) in postmenopausal women with symptoms and signs of urogenital ageing. Am J Obstet Gynecol 1996;174:85–92.
 Nash HA, Brache V, Alvarez-Sanchez F, Jackanicz TM, Harmon TM. Estradiol delivery by vaginal rings: potential for hormone replacement therapy. Maturitas 1997;26:27–33.
 Bachmann G. The clinical platform for the 17b-estradiol vaginal releasing ring. Am J Obstet Gynecol 1998;178:S257–60.  Chien YW. Novel drug delivery systems, 2nd ed. Drugs and the
pharmaceutical sciences, vol. 50, New York: Marcel Dekker, Inc. 1992. p. 565–76 [Chapter 9].
 Chien YW. Novel drug delivery systems, 2nd ed. Drugs and the pharmaceutical sciences, vol. 50, New York: Marcel Dekker, Inc. 1992. p. 3–12, 47–53 [Chapter 9].
 Chien YW, Lambert HJ, Grant DE. Controlled drug release from polymeric devices I: technique for rapid in vitro release studies. J Pharm Sci 1974;63:365–9.
 Chien YW, Jefferson DM, Cooney JG, Lambert HJ. Controlled drug release from polymeric devices V: hydroxy group effect on drug release kinetics and thermodynamics. J Pharm Sci 1979;68:689–93.
 Roseman J. Release of steroids from a silicone polymer. J Pharm Sci 1972;61:46–50.
 Most CF. Some ﬁller effects on diffusion in silicone rubber. J Appl Polym Sci 1970;14:1019–36.
 Flynn GL, Roseman TJ. J Pharm Sci 1971;60:1788–93.  Theeuwes F, Hussain A, Higuchi T. Quantitative analytical
method for determination of drugs dispersed in polymers using differential scanning calorimetry. J Pharm Sci 1974;63:427.  Jones DS. Dynamic mechanical analysis of polymeric systems of
pharmaceutical and biomedical signiﬁcance. Int J Pharm 1999;179:167–78.
 Waters M, Jagger R, Williams K, Jerolimov V. Dynamic mechanical thermal analysis of denture soft lining materials. Biomaterials 1996;17:1627–30.
 Aranguren MI. Crystallization of polydimethylsiloxane: effect of silica and curing. Polymer 1998;39:4897–903.
R.K. Malcolm et al. / Biomaterials 23 (2002) 3589–3594 3594